ISRN Ceramics

Volume 2012 (2012), Article ID 341285, 10 pages

doi:10.5402/2012/341285

Research Article

Effect of Excess Silicon on the Formation of Ti₃SiC₂ Using Free Ti/Si/C Powders Synthesized via Arc Melting

Mohamad Johari Abu, Julie Juliewatty Mohamed, and Zainal Arifin Ahmad

School of Materials and Mineral Resources Engineering, Universiti Sains Malaysia, Engineering Campus, Penang, 14300 Nibong Tebal, Malaysia

Received 12 November 2012; Accepted 28 November 2012

Academic Editors: S. Marinel, W.-C. Oh, and P. Valerio

Copyright © 2012 Mohamad Johari Abu et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

The aim of this study is to investigate the effect of excess silicon on the formation of from free Ti/Si/C powders synthesized via arc melting. The reactant mixture was prepared according to the off-stoichiometric ratio of 3Ti : ()Si : 2C, where (excess Si) varied from 0 to 0.5. Samples were analyzed using X-ray diffractometry (XRD), field-emission scanning electron microscopy (FESEM), and energy-dispersive spectroscopy (EDS). The relative density and porosity of products were calculated using the Archimedes method. Through optimization of the arcing schedules (time) and excess Si amounts, 86.9 wt% of with a relative density of 86% was obtained. For all products, was identified as the main phase, while TiC, , and were identified as secondary phases. grains were in the form of elongated platelets; they were nucleated and grew on the surface of equiaxed TiC grains. The microporosity present in the TiC-equiaxed grains affected the density and porosity of the products.

1. Introduction

Ti₃SiC₂ is a ternary layered carbide known as MAX phase compound due to the formula, where M is a rare-earth transition metal, A is an A-group element (usually IIIA and IVA) in the periodic table, X is C or N, and n is an integer of 1 or 2 or 3 [1]. This ternary compound has unique characteristics that combine merit properties of metals and ceramics [2]. Like metals, it has excellent electrical (~4.5 × 10⁶ Ω−1 m⁻¹) [3] and thermal (~37 W/m·K) [4] conductivities, relatively low hardness (~4 GPa) [1] which makes it easy to machine like common metal or graphite [5, 6], high Young modulus (~325 GPa) [7], and moderate flexural strength (260–600 MPa) [8, 9], it is not susceptible to thermal shock [10], and it has damage tolerance at high temperatures [4]. It also duplicates several ceramic properties such as good oxidation resistance of up to 1400°C [11, 12], relatively low density (~4.52 g/cm³) [1], and high decomposition temperature (~1700°C) [1], and some researchers have also reported that its melting temperature is up to 3000°C [13]. Most detailed descriptions of thermal, electrical, oxidation, mechanical, and chemical properties were given by Barsoum et al. [1–5, 7, 12]. This material shows good promise for use in many structural and high-temperature applications and for wear and corrosion protection. These applications include turbine blade and stators, heavy duty electrical contacts, and bearing.

Ti₃SiC₂ was firstly synthesized as a thin film in 1967 by chemical reaction [14] and in the 1980s by chemical vapor deposition (CVD) [15, 16]. Later, Ti₃SiC₂ was synthesized as a bulk specimen by arc melting [17] or common sintering [18] of elemental Ti–Si–C powders. In the early 1990s, Ti₃SiC₂ single phase was synthesized as a dense specimen from Ti–SiC–C or Ti–Si–TiC powders blended by hot pressing (HP) [19], hot-isostatic pressing (HIP) [9], and reactive hot-isostatic pressing (RHIP) [20]. Unfortunately, these synthesis routes (HP, HIP, and RHIP) require high temperatures (>1400°C), long sintering times (several hours), expensive equipment, and skillful operators for equipment preparation. However, in the 2000s, a rapid solid-solid or solid-liquid reaction (few seconds) synthesis process was developed to produce a near single phase (bulk form) of Ti₃SiC₂. It is a self-ignited or self-sustained reaction where the reactant is exposed to extreme heat and produces a high exothermic reaction [17] with neighboring particles. To be exact, the self-ignition reaction is dependent on the type of heating source (i.e., electric induction, electric charge, laser, and beam) and the mode of combustion (either a combustion that occurs simultaneously or heterogeneously) [21] through a sample volume.

Two types of heating sources are frequently employed in this reaction: electric induction, where the heat is thermally propagated through the sample, that is, self-propagating high-temperature synthesis (SHS) [13, 22–26], thermal explosion (TE) [21], and SHS coupled with hot isostatic pressing (SHS-HIP) [13, 27], and (2) electric-charge, where heat is generated from electrodischarge among particles [28] which is due to the current flowing between two polling sites (anode and cathode), that is, pulse discharge sintering (PDS) [11, 29–31], spark plasma sintering (SPS) [28, 32] or plasma-activated sintering [33–35], arc melting [17], and also from welding methods. Most researchers followed these methods to synthesize Ti₃SiC₂ single phase by using several starting mixtures (e.g., TiH₂/Si/C [14], Ti/Si/C [9, 10, 18–20, 23, 24, 27, 29, 36–47], Ti/SiC/C [25], Ti/Si/TiC [26, 31], and TiC/Si [48]) and varying the composition of the starting reactant powders (e.g., Ti, Si, C, SiC, TiC, Al, etc.). Unfortunately, some of these methods required the assistance of external pressure together with a high-temperature (>1500°C) postannealing step for long sintering times (several hours) to obtain a near single-phase Ti₃SiC₂ [17, 27].

Two alternative routes for reactant powder preparation commonly received by researchers are the use of excess Si addition and the use of either graphite or carbon black powders. By varying the amount of excess Si addition in the reactant mixture of Ti/Si/C powders, most researchers have successfully fabricated a bulk form of Ti₃SiC₂ through self-ignition reaction. However, when the same mixture was used in pressureless self-ignition for both electric induction and electric charge methods, the purity of the Ti₃SiC₂ produced has never exceeded 60 wt% [17, 21, 44]. Therefore, an alternative route which may influence the yield of Ti₃SiC₂ formed is the addition of excess Si in the starting reactant mixture. In most cases, the purity of Ti₃SiC₂ was reported to be very sensitive to any discrepancies in the stoichiometric formulation [27], especially the Si content [9, 18–20, 23, 24, 27, 29, 36–47]. The amount of excess Si has been varied at –0.5 for 3Ti : ()Si : 2C mixture, in order to produce high purity of Ti₃SiC₂ [23, 38, 42]. However, a few authors have found contrasting results [29, 31, 43]. The aim of excess Si addition is to compensate the loss of evaporated Si when the mixture is sintered above 1414°C (i.e., Si melting point) [49], and the deficiency of Si usually favors the formation of TiC [27, 50]. The addition of excess Si is required in self-ignition reactions since the reactant sample has been subjected to extreme temperatures and high heating rates. In most syntheses, TiC and Ti–Si binary phases were always present in the synthesized products [26]. On the other hand, graphite selection is basically used to facilitate the passing of currents through the sample [25], especially when using an electric charge as a heating source. Graphite is more efficient as an electrical and thermal conductor compared to carbon black because the thermal conductivity of graphite (160 Wm−1 K⁻¹) is higher than carbon black (5 Wm−1 K⁻¹) [51].

The only research that used arc melting was done by Arunajatesan and Carim [17] in 1995. They used free Ti/Si/C powders as the starting reactant, and the output was only 58 wt% of Ti₃SiC₂. The amount of Ti₃SiC₂ was increased to 99 wt% when the same product was postannealed in a vacuum furnace for 100 h. However, no research studying the effects of excess Si on the formation of Ti₃SiC₂ using arc melting has been published. This method will offer crucial advantages such as shorter sintering time (within seconds), low energy consumption, yield of high-purity product as the arcing concept is similar to PDS and SPS method, as well as being easy to control since it is associated with the self-sustaining merit from high exothermic reactions. Hence, a synergistic combination of the arc melting method and the variation of excess Si addition amounts is proposed. This option offers great potential for the rapid yielding of Ti₃SiC₂ to above 60 wt%.

Therefore, the objectives of this work is to study the effects of excess Si in the reactant Ti/Si/C mixture powders on the formation of Ti₃SiC₂ and to establish a process route to produce over 60 wt% of Ti₃SiC₂ using the relatively inexpensive and readily available arc melting method.

2. Experimental Details

Commercially available Ti (particle size ~40 μm, 99% purity), Si (~2 μm, 99% purity), and Cg (~2 μm, 99.9% purity) powders from Sigma-Aldrich Inc. were used as the starting raw materials. The reactant mixture was prepared with a stoichiometric ratio according to the following reaction:

where the amount of varied from 0 to 0.5. These raw materials were dry-mixed using a heavy duty high-speed mixer (Fast-Mill FM 2) with ZrO₂ balls. The powder-to-ball ratio was set at 10 : 1, and the materials were mixed for 1 hour. The mixtures were compacted in a stainless steel die (pellet form) with a diameter of 13 mm under 4 tons of load using a cold-pressed machine (Hand Press Hydrotec). The experimental procedure was divided into two stages: Stage 1 which was dedicated to the optimization of the arcing time and Stage 2 which focused on the optimization of excess Si addition. In Stage 1, pellets (3Ti : Si : 2C) were arced using an arc melting apparatus (UNI-ARC D.C. inverter TIG welder model 200C) at a constant arcing current ( = 90 A) [52] for several arcing times ( = 3–90 s), shielded by pressureless high-purity argon gas (99.99%). The distance between the end-tip (anode) of the tungsten electrode to the surface of the pellet (cathode) was fixed at approximately ~5 mm. In Stage 2, pellets containing different amounts of excess Si () were arced at a constant arcing current (90 A) for the optimum arcing time ( that obtained from Stage 1). The amount of excess Si and arcing parameters are listed in Table 1.

Table 1: Details of excess Si and arcing parameters.

Stage
Number of sample
Reactant
Excess Si (x)
Arcing parameters

I (A)
t (s)

1
3Ti + Si + 2C
0
90
3

2
3Ti + Si + 2C
0
90
5

3
3Ti + Si + 2C
0
90
10

4
3Ti + Si + 2C
0
90
15

1
5
3Ti + Si + 2C
0
90
30

6
3Ti + Si + 2C
0
90
45

7
3Ti + Si + 2C
0
90
60

8
3Ti + Si + 2C
0
90
75

9
3Ti + Si + 2C
0
90
90

2
10
3Ti + Si + 2C
0
90

11
3Ti + 1.1Si + 2C
1.1
90

12
3Ti + 1.15Si + 2C
1.15
90
Optimum time as

13
3Ti + 1.2Si + 2C
1.2
90
obtained in stage 1

14
3Ti + 1.25Si + 2C
1.25
90
(denoted as )

15
3Ti + 1.3Si + 2C
1.3
90

16
3Ti + 1.4Si + 2C
1.4
90

17
3Ti + 1.5Si + 2C
1.5
90

Phase composition of the samples was analyzed using an X-ray diffractometry (Bruker AXS D8 Advance) with CuKα radiation operating at 40 kV and 30 mA at a scanning speed of 0.02°/s and a 2 range of 20–90°. The qualitative and quantitative analyses of these XRD profiles were performed using the calibrated standard method (automatic mode: default) using Rietveld refinement of PANalytical X’Pert Highscore Plus software. The expected residual and good of fit () of XRD profiles were recorded as an indicator for refinement quality level. It is noted that the value of should be below 20 while value should be below 4 for good-quality refinement process. The profile errors can be reduced by switching the calibrated standard mode from default to semiautomatic process. The profile error could be reduced to around 5–10%. Morphology of products was observed using field-emission scanning electron microscope (FESEM model SUPRA 35VP ZEISS) equipped with energy-dispersive spectroscopy (EDS). Lastly, the relative density and porosity of arced samples were calculated based on the Archimedes’ method.

3. Results and Discussion

3.1. Stage 1: Optimizing Arcing Time

Figure 1 shows the XRD patterns of compacted 3Ti : Si : 2C powder mixtures after arcing at a constant 90 A for various arcing times (5–90 s). The Ti₃SiC₂ phase peaks (ICSD: 98-005-3834) were clearly seen in all samples, with the main peak located at 2 = 39.5°. Similarly, the presence of TiC (ICSD: 98-011-1108) as the main ancillary secondary phase can be seen from their medium peaks intensities, where the main peak is located at 2 = 41.8°. The intensity of Ti₃SiC₂ peaks increased with increasing arcing times of up to 5 s. Further prolonging the arcing time only reduces the Ti₃SiC₂ content. However, the intensity of TiC peaks is not consistent below 30 s. Peaks of Ti silicides that is, Ti₅Si₃ (ICSD: 98-007-1873) and TiSi₂ (ICSD: 98-001-3102), and free elements (i.e., Ti and C) can also be detected at certain arcing times. No and Ti₅Si₃ peaks were observed, as was claimed by El-Raghy and Barsoum [53] and Wu et al. [54]. They proposed that Ti₅Si₃ forms firstly at 800–1400°C. In this work, the corresponding peaks of TiCx and Ti₅Si₃ were proven as TiC and Ti₅Si₃; due to the presence of fine C in the Ti/Si/C system, the rapid reaction between Ti-melt and C produced TiC. The high stability of TiC present clarifies that its decomposition is not likely to occur at low temperatures. Therefore, it is reasonable to propose that the first compounds to appear were TiC and Ti₅Si₃, instead of Ti and Ti₅Si₃. As compared to Ti₃SiC₂, the intensity of the Ti₃SiC₂ peaks is higher than TiC and Ti₅Si₃; hence, the formation rate of Ti₃SiC₂ is higher than that of TiC and Ti₅Si₃. The pulse-discharge arcing in the sample is believed to have occurred at temperatures higher than 1400°C. However, TiSi₂, Ti, and C were observed at 75 and 90 s, corresponding to the decomposition of Ti₅Si₃. Therefore, it is believed that arcing at longer times (>75 s) only leads to the production of TiSi₂, Ti, and C which are the decomposition products of Ti₃SiC₂ and/or Ti₅Si₃.

Figure 1: XRD patterns of compacted 3Ti/Si/2C powders arced at a constant 90 A for various arcing times (3–90 s).

Table 2 summarizes the results of compacted Ti/Si/C mixture produced using the arc melting method. The different arcing time (3–90 s) was identified as the arcing parameter. All results are listed with values of (<12.6) and (<3.4), which indicate good refinement processes. In all cases, the products were formed in two main phases, that is, Ti₃SiC₂ and TiC, consisting of small composition of other phases such as Ti₅Si₃, TiSi₂, Ti, and C. The Ti₃SiC₂ composition percentage of the as-synthesized samples arced at 5 s was higher than other arcing schedules. The highest Ti₃SiC₂ percentage in sample number 2 was 62.2 wt%. This demonstrates the significant effect of arcing time on the Ti₃SiC₂ formation. However, the lattice parameters of these synthesized samples were not consistent to each other. This was due to the difficulty of arcing control because of the exothermic reaction.

Table 2: Results obtained by different arcing parameters.

Stage
No.
Reactant
Arcing parameters
Phases detected (weight fraction, wt%)
Lattice parameters Ti₃SiC₂

I (A)
t (s)
Ti₃SiC₂
TiC
Ti₅Si₃
TiSi₂
Ti
C

S
a = b ()
c ()

1
3Ti + Si + 2C
90
3
50.1
27.6
22.3
—
—
—
10.378
2.412
3.0660
17.6300

2
3Ti + Si + 2C
90
5
62.2
37.8
—
—
—
—
11.418
2.068
3.0715
17.6900

3
3Ti + Si + 2C
90
10
55.7
34.0
10.7
—
—
—
10.236
2.476
3.0786
17.6849

4
3Ti + Si + 2C
90
15
53.3
30.0
10.3
—
—
—
12.638
2.327
3.0669
17.6640

1
5
3Ti + Si + 2C
90
30
54.0
23.1
—
12.3
—
—
10.171
3.380
3.0666
17.6406

6
3Ti + Si + 2C
90
45
42.7
33.1
24.3
—
—
—
11.077
2.285
3.0679
17.6440

7
3Ti + Si + 2C
90
60
35.7
56.9
7.4
—
—
—
11.558
2.676
3.0680
17.6690

8
3Ti + Si + 2C
90
75
29.4
57.8
—
4.2
1.8
0.2
12.423
2.188
3.0694
17.6775

9
3Ti + Si + 2C
90
90
23.1
60.4
13.7
—
2.7
—
12.004
1.976
3.0644
17.6505

Figure 2 shows the weight percentage, relative density, and porosity of samples of Ti₃SiC₂ and TiC phases, arced at a constant 90 A for various arcing times (3–90 s) in accordance to Table 2. The Ti₃SiC₂ phase was obviously formed at a short arcing time (~5 s). Initially, from 3 s to 5 s, the Ti₃SiC₂ content changed slightly and reached a maximum at 5 s. As arcing time was increased to above 5 s, Ti₃SiC₂ decreased; this implies that the optimal arcing time () for Ti₃SiC₂ formation from compacted 3Ti/Si/2C powders is 5 s. The Ti₃SiC₂ yield in this study is superior compared to that produced in previous work reported by Khoptiar and Gotman [21] which yielded only 45 wt% Ti₃SiC₂ using free postannealed thermal explosion. However, the TiC content was similar to Ti₃SiC₂ content at the lower arcing time of 30 s. The results showed a reverse trend when arcing time was prolonged to above 30 s. The trend in porosity is very much proportional to the amount of TiC phases present. The relative density of all samples was within the range of 82.9–87.5% and showed the reverse of the trend in porosity.

Figure 2: Effects of soaking times on the relative density, porosity, and phases detected (wt%).

Figure 3 shows FESEM micrographs (as observed at dense polished sample surface and porous site) of a sample arced at 90 A for 5 s. At least two types of grains can be seen: elongated platelets and equiaxed grains. The grain size of the elongated platelets (i.e., thickness) is 1–8 μm, while the equiaxed grain size is about 2–16 μm. They are surrounded by the irregular appearance of the melt region. Identification of grains was confirmed using EDX analysis. As shown in Figure 3(a), the elongated platelets and equiaxed grains can be identified as Ti₃SiC₂ and TiC, respectively, while TiSi₂ and/or Ti₅Si₃ is the melt region. These micrographs confirm the nucleation and growth of Ti₃SiC₂ within the TiC grains (Figure 3(b)), which is similar to the observation made by previous researchers [49]. However, it can be obviously seen that Ti₃SiC₂ formed on the surface of TiC grains. This directly proves that Ti₃SiC₂ formation on TiC surface is possible. It is marked as an interface of Ti-Si and TiC grains. Therefore, the interface between them is governed by Ti₃SiC₂ formation, as similarly reported by Riley et al. [24]. However, the nucleation and growth of Ti₃SiC₂ within the Ti₅Si₃ grains are unclear. Microporosity appeared within the TiC grains. This is in agreement with Li et al. [36] who reported that the flame front (combustion) of the heat propagation was not completed and C was diffused into the Ti site to form Ti, leaving a large amount of microporosity inside the grains. The arrow in Figure 3(a) also refers to the microporosity obtained in TiC grains. Meanwhile, Figure 3(b) confirms that no micro-porosity was seen on the surface of this TiC grain.

(a)

(b)

Figure 3: FESEM morphology of sample ( = 0) scanned at (a) the dense surface and (b) pore site after arcing at a constant 90 A for 5 s.

3.2. Stage 2: Optimizing Excess Si Addition

Figure 4 shows XRD patterns of excess Si samples after arcing at a constant 90 A for 5 s. It is found that the varying amount of excess Si in the reactant mixture directly influenced the Ti₃SiC₂ yield. This can be seen from the intensity of the main Ti₃SiC₂ peak (2 = 39.5°). The strongest peak can be observed for the sample with excess Si of . It is proposed that the presence of sufficient Si produces a large wetting area in the compacted mixture which reacts with Ti to form the Ti–Si melt region. This Ti–Si reacts with TiC to form Ti₃SiC₂, which is in agreement with a previous study conducted by Riley et al. [24]. However, as increased, the peak intensity of Ti₃SiC₂ decreased. This phenomenon was due to too much Si melt region surrounding the coarse Ti and C dispersed from the Ti surface. This is proven by the weak intensity of TiC peaks observed.

Figure 4: XRD patterns of compacted 3Ti/Si/2C powders after arcing at a constant 90 A for 5 s.

TiC is the main secondary phase present in all samples, along with the TiSi₂ melt region. However, small peaks of Ti₅Si₃ are only present in certain samples. The weak intensity of both TiSi₂ and TiC peaks indicate that TiSi₂ and TiC may react with each other to form Ti₃SiC₂. Therefore, the addition of excess Si was favorable in producing TiSi₂ instead of Ti₅Si₃. Further additions () have clearly lowered the peak intensities of Ti₅Si₃, α-Ti, and C. It seems that it does not influence the Ti₃SiC₂ formation; instead, it was responsible for lowering intensities of Ti₃SiC₂ peaks. Hence, it is proposed that the low peak intensity of α-Ti present in this sample is affected by thermal activities which can be explained using two assumptions.

Firstly, the physical and electrical properties of Si powder are, respectively, smaller and weaker compared to those of Ti. Therefore, Si will stick onto the surfaces of Ti particles after the mixing and milling process; this produces resistance/barrier against current flow. Secondly, Si is classified as a good thermal conductor; hence it produces large melt regions on the surfaces of Ti particles since it has the lowest melting temperature (~1414°C) [49] in the Ti–Si–C system. Therefore, small C particles will partly diffuse into the Si melt region, while others will be trapped in the same region and are not able to react with the Ti phase to form TiC. This assumption may be relevant as well as for α-Ti and C phases which were observed in samples containing . It is proposed that the medium intensity of the Ti₃SiC₂ peaks is affected by the direct reaction between the TiC and Si melt. This is a reasonable assumption as Ti–Si presented low peak intensity.

Table 3 shows the results (phases percentage and lattice parameters) of compact excess Si samples arced at a constant 90 A for 5 s. The highest composition of Ti₃SiC₂ (86.9 wt%) was obtained from the reaction system of 3Ti/1.2Si/2C. The value of Ti₃SiC₂ composition is parallel to the XRD pattern of sample number 13, as shown in Figure 4. Figure 5 shows the quantitative XRD analysis of phase percentage (Ti₃SiC₂, TiC, and TiSi₂), relative density, and porosity of the synthesized samples, performed according to Rietveld refinement and calculated based on the Archimedes method, respectively. 86.9 wt% of Ti₃SiC₂ was successfully synthesized from excess Si () sample. Therefore, the optimum degree of Ti₃SiC₂ phase formation is from the product with excess Si (). Figure 5 also shows the reverse effect for both TiC and Ti₃SiC₂ at a relatively different . An addition of excess Si in Ti/Si/C only improves the content of TiSi₂ in the silicides melt region. Therefore, the formation of new silicides in the products should not be favored, which is in accordance with the work done by Zhang et al. [31]. The relative density of all samples with excess Si ranges between 85.19 and 86.25%, and the porosity is shown to be directly proportional to the amount of TiC present. Therefore, it is suggested that the addition of excess Si does not effectively increase the relative density of the product. On the other hand, it increased the amount of porosity in TiC grains.

Table 3: Results obtained by different excess Si contents in starting reactant.

Stage
No.
Reactants
Arcing parameters
Phases detected (weight fraction, wt%)
Lattice parameters Ti₃SiC₂

I (A)
t (s)
Ti₃SiC₂
TiC
Ti₅Si₃
TiSi₂
α-Ti
C

S
a = b ()
c ()

2
10
3Ti + Si + 2C
90
5
62.2
37.8
—
—
—
—
11.418
2.068
3.0715
17.6900

11
3Ti + 1.1Si + 2C
90
5
74.2
24.9
—
0.9
—
—
10.418
2.068
3.0681
17.6657

12
3Ti + 1.15Si + 2C
90
5
76.7
21.2
—
2.1
—
—
12.432
1.443
3.0699
17.6860

13
3Ti + 1.2Si + 2C
90
5
86.9
9.4
—
3.8
—
—
12.619
2.326
3.0686
17.6746

14
3Ti + 1.25Si + 2C
90
5
64.6
30.4
—
5.0
—
—
11.767
1.384
3.0718
17.6887

15
3Ti + 1.3Si + 2C
90
5
56.1
32.0
—
11.9
—
—
11.569
2.447
3.0689
17.6680

16
3Ti + 1.4Si + 2C
90
5
54.6
41.3
—
2.7
0.4
1.0
10.292
1.258
3.0694
17.6920

17
3Ti + 1.5Si + 2C
90
5
30.0
47.8
4.0
6.2
1.7
1.3
12.848
2.806
3.0666
17.6407

Figure 5: Effects of excess Si on the relative density, porosity, and phases detected (wt%).

Figure 6 shows the FESEM micrographs of as-polished samples arced at 90 A for 5 s with varying excess Si content in the mixture. The different amounts of Si added into the mixture affected the Ti₃SiC₂ grain size and distribution. Typically, the thickness of Ti₃SiC₂ grain size is 1–15 μm. The largest Ti₃SiC₂ grain size was obtained in the sample with excess Si (). Further additions of excess Si () into the reactant mixture were responsible for reducing Ti₃SiC₂ grain size and its depletion into small pieces. Its effect on the equiaxed (TiC) grain size is inversely proportional to Ti₃SiC₂. The melt region that surrounds the elongated platelet and equiaxed grains most likely belongs to TiSi₂ melt, which was formed as a necessary intermediate phase in the formation and decomposition of Ti₃SiC₂. It is observed that the area of TiSi₂ melt is magnified on the equiaxed grains. Therefore, it is possible that a reaction would occur between the melt region and TiC in Ti₃SiC₂ formation. It is proposed that large areas of TiSi₂ melt region on TiC surfaces produce a large amount of elongated grains. This is possible because the ignition temperature is >1400°C, which is close to the melting temperature of Si. The goal of adding excess Si is to compensate the loss of Si in the system, which agrees with a finding from a study done by Yang et al. [49]. From the discussion above, it is suggested that excess Si can be regarded as a favorable additional element to synthesize 86.9 wt% of Ti₃SiC₂ at a relatively short time, using the arc melting method. The micrograph in Figure 6(f) is an example of microporosity that exists in the equiaxed TiC grain.

(a)

(b)

(c)

(d)

(e)

(f)

(g)

(h)

Figure 6: FESEM micrograph of as-polished samples containing different content of excess Si; (a) , (b) , (c) , (d) , (e) , (f) , (g) , and (h) arced at a constant 90 A for 5 s.

4. Conclusion

86.9 wt% of Ti₃SiC₂ was successfully synthesized from compacted 3Ti/1.2Si/2C powders arced at 90 A for 5 s. It is an improvement of approximately 44% from the yield produced in the study conducted in 1995 using pressureless self-ignition reaction. Ti₃SiC₂ was formed as the main phase and TiC as the main secondary phase, whereas TiSi₂ and Ti₅Si₃ were formed as secondary melt region phase. Based on product morphology, elongated platelets of Ti₃SiC₂ were found nucleated and grown on the surfaces of equiaxed TiC grains. However, these TiC grains contain a lot of microporosity which relatively affects the density and porosity of products.

Acknowledgments

This work was supported by the National Science Fund of Malaysia (NSF) under Grant no. 060105SF0441, Research University Individual (RUI) under Grant no. 1001/PELECT/814117, and Malaysian Ministry of Higher Education scholarship (MyBrain15). The authors would like to thank all members of the Ceramic Laboratories at the School of Materials and Mineral Resources Engineering, Universiti Sains Malaysia, and technicians for their assistance and helpful discussion.

References

M. W. Barsoum, “ phases: a new class of solids: thermodynamically stable nanolaminates,” Progress in Solid State Chemistry, vol. 28, no. 1–4, pp. 201–281, 2000.

M. W. Barsoum and T. El-Raghy, “Synthesis and characterization of a remarkable ceramic: ,” Journal of the American Ceramic Society, vol. 79, no. 7, pp. 1953–1956, 1996.

M. W. Barsoum, H. I. Yoo, I. K. Polushina, Y. V. Rud, and T. El-Raghy, “Electrical conductivity, thermopower, and Hall effect of , , and ,” Physical Review B, vol. 62, no. 15, pp. 10194–10198, 2000.

M. W. Barsoum, T. El-Raghy, C. J. Rawn et al., “Thermal properties of ,” Journal of Physics and Chemistry of Solids, vol. 60, no. 4, pp. 429–439, 1999.

M. W. Barsoum, D. Brodkin, and T. El-Raghy, “Formation and thermal stability of amorphous Ti-Si-C alloys,” Scripta Materialia, vol. 36, no. 5, pp. 535–541, 1997.

Y. Zhang, G. P. Ding, Y. C. Zhou, and B. C. Cai, “: a self-lubricating ceramic,” Materials Letters, vol. 55, no. 5, pp. 285–289, 2002.

M. W. Barsoum and T. El-Raghy, “A progress report on , , and the H-phases, M₂BX,” Journal of Materials Synthesis and Processing, vol. 5, no. 3, pp. 197–216, 1997.

Y. C. Zhou and Z. M. Sun, “Microstructure and mechanism of damage tolerance for bulk ceramics,” Materials Research Innovations, vol. 2, no. 6, pp. 360–363, 1999.

N. F. Gao, Y. Miyamoto, and D. Zhang, “Dense prepared by reactive HIP,” Journal of Materials Science, vol. 34, no. 18, pp. 4385–4392, 1999.

M. Naka, H. Sakai, M. Maeda, and H. Mori, “Formation and thermal stability of amorphous Ti-Si-C alloys,” Materials Science and Engineering A, vol. 226–228, pp. 774–778, 1997.

Z. M. Sun, Z. F. Zhang, H. Hashimoto, and T. Abe, “Ternary compound : Part I: pulse discharge sintering synthesis,” Materials Transactions, vol. 43, no. 3, pp. 428–431, 2002.

M. W. Barsoum, T. El-Raghy, and L. Ogbuji, “Oxidation behavior of in the temperature range of 900°C–1400°C,” Journal of the Electrochemical Society, vol. 144, no. 7, pp. 2508–2516, 1997.

R. Pampuch, J. Lis, L. Stobierski, and M. Tymkiewicz, “based materials produced by self-propagation high-temperature synthesis (SHS) and ceramic processing,” Journal of the European Ceramic Society, vol. 5, no. 5, pp. 283–287, 1989.

W. Jeitschko and H. Nowotny, “Diffraction thermometry and differential thermal analysis,” Monatshefte für Chemie, vol. 98, pp. 329–337, 1967.

T. Goto and T. Hirai, “Chemically vapor deposited ,” Materials Research Bulletin, vol. 22, no. 9, pp. 1195–1201, 1987.

J. J. Nickl, K. K. Schweitzer, and P. Luxenberg, “Gasphasenabscheidung im system Ti-C-Si,” Journal of The Less Common Metals, vol. 26, no. 3, pp. 335–353, 1972.

S. Arunajatesan and A. H. Carim, “Synthesis of titanium silicon carbide,” Journal of the American Ceramic Society, vol. 78, no. 3, pp. 667–672, 1995.

C. Racault, F. Langlais, and R. Naslain, “Solid-state synthesis and characterization of the ternary phase ,” Journal of Materials Science, vol. 29, no. 13, pp. 3384–3392, 1994.

L. Yongming, P. Wei, L. Shuqin, C. Jian, W. R. Gang, and L. Jianqiang, “Synthesis of high-purity polycrystals by hot-pressing of the elemental powders,” Materials Letters, vol. 52, no. 4-5, pp. 245–247, 2002.

T. El-Raghy and M. W. Barsoum, “Processing and mechanical properties of : I, Reaction path and microstructure evolution,” Journal of the American Ceramic Society, vol. 82, no. 10, pp. 2849–2854, 1999.

Y. Khoptiar and I. Gotman, “Synthesis of dense -based ceramics by thermal explosion under pressure,” Journal of the European Ceramic Society, vol. 23, no. 1, pp. 47–53, 2003.

A. G. Merzhanov, “Self-propagating high-temperature synthesis: non-equilibrium processes and equilibrium products,” Advance in Science and Technology, vol. 45, pp. 36–44, 2006.

J. Lis, R. Pampuch, T. Rudnik, and Z. Wȩgrzyn, “Reaction sintering phenomena of self-propagating high-temperature synthesis-derived ceramic powders in the Ti-Si-C system,” Solid State Ionics, vol. 101–103, no. 1, pp. 59–64, 1997.

D. P. Riley, E. H. Kisi, T. C. Hansen, and A. W. Hewat, “Self-propagating high-temperature synthesis of : I, ultra-high-speed neutron diffraction study of the reaction mechanism,” Journal of the American Ceramic Society, vol. 85, no. 10, pp. 2417–2424, 2002.

C. L. Yeh and Y. G. Shen, “Effects of SiC addition on formation of by self-propagating high-temperature synthesis,” Journal of Alloys and Compounds, vol. 461, no. 1-2, pp. 654–660, 2008.

C. L. Yeh and Y. G. Shen, “Effects of TiC addition on formation of by self-propagating high-temperature synthesis,” Journal of Alloys and Compounds, vol. 458, no. 1-2, pp. 286–291, 2008.

J. Lis, Y. Miyamoto, R. Pampuch, and K. Tanihata, “-based materials prepared by HIP-SHS techniques,” Materials Letters, vol. 22, no. 3-4, pp. 163–168, 1995.

N. F. Gao, J. T. Li, D. Zhang, and Y. Miyamoto, “Rapid synthesis of dense by spark plasma sintering,” Journal of the European Ceramic Society, vol. 22, no. 13, pp. 2365–2370, 2002.

Z. F. Zhang, Z. M. Sun, H. Hashimoto, and T. Abe, “Application of pulse discharge sintering (PDS) technique to rapid synthesis of from Ti/Si/C powders,” Journal of the European Ceramic Society, vol. 22, no. 16, pp. 2957–2961, 2002.

Z. M. Sun, S. Yang, and H. Hashimoto, “ powder synthesis,” Ceramics International, vol. 30, no. 7, pp. 1873–1877, 2004.

Z. F. Zhang, Z. M. Sun, H. Hashimoto, and T. Abe, “Effects of sintering temperature and Si content on the purity of synthesized from Ti/Si/TiC powders,” Journal of Alloys and Compounds, vol. 352, no. 1-2, pp. 283–289, 2003.

B. Y. Liang, S. Z. Jin, and M. Z. Wang, “Low-temperature fabrication of high purity ,” Journal of Alloys and Compounds, vol. 460, no. 1-2, pp. 440–443, 2008.

S. H. Risbud and J. R. Groza, “Clean grain boundaries in an aluminum nitride ceramic densified without additives by a plasma-activated sintering process,” Philosophical Magazine B, vol. 69, pp. 525–533, 1994.

J. A. Schneider, S. H. Risbud, and A. K. Mukherjee, “Rapid consolidation processing of silicon nitride powders,” Journal of Materials Research, vol. 11, no. 2, pp. 358–362, 1996.

M. J. Tracy and J. R. Groza, “Consolidation of nanocrystalline Nb-Al powders by plasma activated sintering,” Nanostructured Materials, vol. 2, no. 5, pp. 441–449, 1993.

J. F. Li, F. Sato, and R. Watanabe, “Synthesis of polycrystals by hot-isostatic pressing of the elemental powders,” Journal of Materials Science Letters, vol. 18, no. 19, pp. 1595–1597, 1999.

F. Sato, J. F. Li, and R. Watanabe, “Reaction synthesis of from mixture of elemental powders,” Materials Transactions, vol. 41, no. 5, pp. 605–608, 2000.

R. Radhakrishnan, J. J. Williams, and M. Akinc, “Synthesis and high-temperature stability of ,” Journal of Alloys and Compounds, vol. 285, no. 1-2, pp. 85–88, 1999.

Y. Zhou, Z. Sun, S. Chen, and Y. Zhang, “In-situ hot pressing/solid-liquid reaction synthesis of dense titanium silicon carbide bulk ceramics,” Materials Research Innovations, vol. 2, no. 3, pp. 142–146, 1998.

Z. M. Sun and Y. C. Zhou, “Fluctuation synthesis and characterization of fiber-like powders,” Materials Research Innovations, vol. 2, no. 4, pp. 227–231, 1998.

M. A. El-Saeed, F. A. Deorsola, and R. M. Rashad, “Optimization of the MAX phase synthesis,” International Journal of Refractory Metals and Hard Materials, vol. 35, pp. 127–131, 2012.

H. Li, L. M. Peng, M. Gong, J. H. Zhao, L. H. He, and C. Y. Guo, “Preparation and characterization of powder,” Ceramics International, vol. 30, no. 8, pp. 2289–2294, 2004.

S. B. Li, H. Zhai, Y. Zhou, and Z. L. Zhang, “Synthesis of powders by mechanically activated sintering of elemental powders of Ti, Si and C,” Materials Science and Engineering A, vol. 407, no. 1-2, pp. 315–321, 2005.

Y. Kuang, N. Tungwai leo, C. Hu, and Y. Li, “Effect of Si content on the synthesis of bulk material by pressureless sintering,” Materials Science Forum, vol. 610–613, pp. 1263–1267, 2009.

C. S. Park, F. Zheng, S. Salamone, and R. K. Bordia, “Processing of composites in the Ti-Si-C system,” Journal of Materials Science, vol. 36, no. 13, pp. 3313–3322, 2001.

V. Gauthier, B. Cochepin, S. Dubois, and D. Vrel, “Self-propagating high-temperature synthesis of : study of the reaction mechanisms by time-resolved X-ray diffraction and infrared thermography,” Journal of the American Ceramic Society, vol. 89, no. 9, pp. 2899–2907, 2006.

S. B. Li, J. X. Xie, L. T. Zhang, and L. F. Cheng, “Synthesis and some properties of by hot pressing of titanium, silicon, and carbon powders—part 1: effect of starting composition on formation of and observation of crystal morphology,” Materials Science and Technology, vol. 19, no. 10, pp. 1442–1446, 2003.

I. Kero, M. L. Antti, and M. Oden, “Synthesis of by Reaction of TiC and Si Powders,” in Proceedings of the 32nd International Conference on Advanced Ceramic and Composites Site, pp. 1–20, Daytona Beach, Fla, USA, January 2008.

S. Yang, Z. M. Sun, and H. Hashimoto, “Reaction in powder synthesis from a Ti-Si-TiC powder mixture,” Journal of Alloys and Compounds, vol. 368, no. 1-2, pp. 312–317, 2004.

X. Tong, T. Okano, T. Iseki, and T. Yano, “Synthesis and high temperature mechanical properties of /SiC composite,” Journal of Materials Science, vol. 30, no. 12, pp. 3087–3090, 1995.

R. L. Powell and G. E. Childs, American Institute Physics Handbook, New York, NY, USA, 1972.

J. J. Mohamed, P. C. Hung, and Z. A. Ahmad, “Synthesis of via modified-SHS system through arc melting,” Advanced Materials Research, vol. 239–242, pp. 2128–2131, 2011.

T. El-Raghy and M. W. Barsoum, “Diffusion kinetics of the carburization and silicidation of ,” Journal of Applied Physics, vol. 83, no. 1, pp. 112–119, 1998.

E. Wu, D. P. Riley, E. H. Kisi, and R. I. Smith, “Reaction kinetics in synthesis studied by time-resolved neutron diffraction,” Journal of the European Ceramic Society, vol. 25, no. 15, pp. 3503–3508, 2005.